Home >Documents >2014-1-43- p Bending Stiffness of Knitted Fabrics Ndash; Nbsp;Comparison of Test Methods p

Date post: | 23-Dec-2015 |

Category: | ## Documents |

View: | 13 times |

Download: | 1 times |

Share this document with a friend

Description:

Statistical Analyses and Propertiesof Viloft/Polyester and Viloft/Cotton BlendedRing-Spun Yarns

Transcript:

Goetzendorf-Grabowska B, Karaszewska A, Vlasenko VI., Arabuli AT. Bending Stiffness of Knitted Fabrics Comparison of Test Methods.FIBRES & TEXTILES in Eastern Europe 2014; 22, 1(103): 43-50.

43

Bending Stiffness of Knitted Fabrics Comparison of Test Methods

Bogna Goetzendorf-Grabowska, Agnieszka Karaszewska,

*Victoria I. Vlasenko, *Arsenii T. Arabuli

Textile Research Institute, Scientific Department

of Unconventional Technologies and Textiles, ul. Brzeziska 5/15, 92-103 d, Poland

E-mail: [email protected]

*Kiev National University of Technologies & Design,

2N-Danchenko St.korp. 1, 132 01011, Kiev, Ukraine

AbstractThe bending stiffness of a textile is a feature determining comprehensive indicators such as fabric drapability and handle. Most methods of assessing the bending stiffness of textiles are based on the principle of the determination of the strain and force dependence. The simplest are methods involving the unidirectional straining force, which do not consider the anisotropy of the fabrics physical properties. However, methods that allow the deter-mination of multi-directional stiffness provide a more complete assessment. The aim of this work was to comparatively evaluate three testing methods that utilise different measure-ment principles. The experimental design included a unidirectional force action (PN-73/P0431), multidirectional force action (ASTM-D 4032-94), and bending stiffness testing by the direct determination of Youngs modulus by the method used at Kiev University. The methods analysed were assessed by statistical tests. Knitted fabrics with a net stitch were used as the test materials.

Key words: test methods, bending stiffness, statistic test.

ing. The most popular gravimetric meth-ods are those using the determination of the bending length as a measure of the interaction between fabric weight and stiffness [7 - 11]. One of them is Pierces Heard Loop Test [12]. This principle is used by ASTM [8] and PN [11]. A known example of the bending length prin-ciple is the Cantilever Test for Stiffness [13, 14].

The determination of fabric stiffness is also included in KES (Kawabata Evalua-tion System) and Handle-O-Meter Tester [15 - 19].

The simplest and most available methods are based on the unidirectional action of the straining force action [19, 20]. In view of the anisotropy of physical properties of textile fabrics, the method of the uni-directional action of force usually takes into account three basic directions of the fabric (longitudinal, transversal and the bias- 45 (deg) to the samples axis). This is, however, a simplification that does not include the anisotropy character. The methods that determine multidirectional stiffness give a more complete assess-ment [21 - 26].

An interesting method has been devel-oped at the Kiev National University of Technologies & Design (Ukraine) for the dynamic determination of elasticity mod-ulus (Ed) based on a theory that elasto-plastic bodies subjected to cyclic sinusoi-dal stresses reach a state of equilibrium after a number of cycles, which is a func-tion of the structures dynamic proper-ties [27]. A similar method of measuring Youngs module for fibre was developed by Polish authors [28].

Isotropic materials are characterised by one Youngs modulus, while for aniso-tropic materials such as textiles, the num-ber of elasticity coefficients is higher than one, which are connected with the main anisotropy directions. Due to the com-plex fibre structure, the action of external forces results in complicated phenomena of mechanical properties that cannot be included in the classic theory of an elas-tic or plastic body. Taking into account the components of strain occurring under the influence of force, fibres are defined as anisotropic visco-elastic bodies [5]. The complexity of the fabric strain anisotropy results from the overlapping parameters of the structures of fibres, yarns and fabrics.

There are many test methods known for measuring fabric bending stiffness, but only few of them use Youngs modulus as a basis for measuring stiffness [2].

Most methods described and used in tex-tile laboratories are based on the princi-ple of indirect stiffness assessment by determining the dependence of strain and the force that induces this strain. Some methods use tensile testing machines for precise measurement of the dependence of the force and strain of flat textile fab-rics [6]. In view of the narrow range of the acting forces and occurring strains, such methods allow one to obtain results with smaller errors.

Dziworska [2] introduced two types of testers for measuring bending stiffness. The first type of testers measure the fab-ric strain under its own weight (gravita-tion method), whereas the other testers are based on the measurements of forces, bending moments or energy during bend-

n IntroductionThe stiffness of some fabrics constitutes the basic feature determining their suit-ability for a specific use. The bending stiffness of textiles has become a funda-mental property in determining the com-plex parameter of fibre or fabric drapabil-ity and handle.

The drapeability of textiles in physical terms is a result of mutual interaction between the bending stiffness and fabric weight [1, 2].

Generally rigidity is defined as the capa-bility of a material to resist strain under the influence of different forces such as compression, uniaxial tension, bending, simple shearing or vibration [3]. For elastic bodies, in most strains, stiffness is characterised by Youngs modulus (E), determined as the modulus of linear strain ability [4]. This is a parameter de-termining fabric elasticity, which makes the material linear strain dependent on stress occurring in it according to the de-pendence:

E = /, N/m2 (1)

where: - relative linear strain, - stress

The stiffness rigidity (G) is measured by the product of modulus (E) and the mo-ment of inertia (I) of the cross-section in relation to the neutral axis passing through the middle of the cross-section according to the following formula:

G = E I, N (2)

This dependence constitutes a theoretical basis for the physical determination of the bending rigidity parameter [1].

FIBRES & TEXTILES in Eastern Europe 2014, Vol. 22, No. 1(103)44

The aim of this work was to comparative-ly evaluate three selected testing methods using different measurement principles to evaluate the bending stiffness of net-like warp knitted fabrics.

The test material consisted of 10 groups of surgical netlike warp knitted fabrics with various variants of yarn and knitting stitches of the same fibre raw material (polyester).

The experimental design includes uni-directional force action (PN-73/P0431) and multidirectional force action (ASTM-D 4032-94) as well as bending stiffness testing by direct determination of Youngs modulus by the method used at Kiev University.

Comparison of results and properties of the methods evaluated was carried out by means of statistical tests [29 - 32].

n Experimental detailsMaterialTest materials consisted of polyester openwork warp knitted fabrics with dif-ferent fabric and yarn parameters. Basic fabric parameters and images of knitting stitches are listed in Table 1 and shown in Figure 1.

To better characterise the structure of the net knitted fabrics tested, the following parameters were determined on the basis of microscopic analysis [33]:Cs total - Total surface of voids - the sum

of surfaces of all the voids on the sample surface tested Ss in mm2

Cs max. - Maximal surface of a single void in mm2, Figure 2.

P - Porosity - the percentage content of the total void surface in the sample surface

P = Cs total/Ss, % (3)

The results of this analysis are listed in Table 2.

MethodsDetermination of textile fabric stiffness - Polish Standard PN-73/P0463 [11]This is a gravitational method based on Pierces theory. The principle of this method consists in measuring the bend-ing length of a sample, whose both ends are fixed in a clamp. The freely hanging sample forms a heard loop, and the sag length in m is the basis for determination

Table 1. Characteristics of test materials.

Symbol of knitted

fabric group

Type of yarn Type of knitting stitch

Fabric structure,

number /cmWeight,

g/m2 wale course

I Polyester30 dtex, f 1

Plain, double needle board stitch with combined stitches (velvet, chain)

16.3 11.8 54.0II 20.0 12.0 65.2

III Polyester56 dtex f 24 Double Plain, double needle board stitch with network structure

22.1 11.2 62.6

IV Polyester56 dtex f 24 Single 21.8 10.9 41.9

V Polyester56 dtex f 24 Double Plain, three needle board, stitch with network structure

16.9 11.6 67.5

VI Polyester56 dtex f 24 Single 18.0 12.1 49.5

VII

Polyester30 dtex f 1

Plain, double needle board stitch with network structure

19.6 10.7 22.2VIII 24.6 11.8 27.2IX Plain, double needle board stitch,

with network structure 28.2 9.5 24.7

X 29.7 11.2 28.3

Figure 1. Images of knitting stitches.

Figure 2. Surface of a single void of an exemplary sample.

Plain, double needle board stitch, with combined stitches (velvet, chain)

I II

III IV IX X

V VI

VII VIII

Plain stitch, double needle board with a network structure

Plain, three needle board stitch with a network structure

Plain, double needle board stitch

Sample VCs max: 3.118 mm2

P: 50.9%

45FIBRES & TEXTILES in Eastern Europe 2014, Vol. 22, No. 1(103)

nance occurs. The numerical value of Tp appears on the frequency meter at the moment of resonance.

The low frequency generator determines the frequency of oscillation at resonance, and the frequency meter gives the nu-merical value of the period, Tp. It is the numerical value of the period that is used for further calculations.

Schema of the Stiffness Tester, shown in Figure 4.

The force F, N required to push out a sample along the holes axis at a length of 57 mm is a result of measurement. An electronic meter with a memory element allows a read-out of 10 measurements with statistics. Stiffness measurements were performed according to the proce-dure of the above standard for sample size n = 10.

Dynamic modulus of elasticity Ed (method UDM-1) [27]Tests of bending stiffness based on the determination of Youngs modulus were carried out at Kiev National University of Technology & Design. The UDM-1 apparatus operating on the principle of inducing the resonance of the samples longitudinal vibration and measuring the vibration frequency at the moment of equilibrium allows one to determine the elasticity modulus. A scheme of this ap-paratus is shown in Figure 5.

The dynamic modulus of elasticity is de-termined on the basis of the sample vi-bration and parameters (dimension and weight). The samples were loaded with a given mass MI depending on the type of fabrics tested. Under the influence of this load samples were investigated. Free longitudinal damped oscillations occur in the sample due to the given load. Oscilla-tions depend on the properties of the ma-terials, in particular its elasticity.

To determine the oscillation period, Tp, one must determine the oscillation frequency of the sample. This can be achieved by turning the handle of the generator at the frequency which reso-

of the bending length. Figure 3 shows the scheme of measurement.

The loop length m allows determination of the bending length c on the basis of tabulated values c = f (m)

Based on the measurement results, the bending stiffness, G, is determined:

G = 10-6mFc3g, mNm (mNm - milinewton meter) (4)

where: mF fabric weight, g/m2, c bending length, cm, g acceleration of gravity, m/s2.

Bending modulus q is calculated from the formula:

q = 1.2104G/h, kPa (5)

where: h sample thickness, mm.

Measurements are separately performed for the longitudinal and transversal direc-tions and the result is the geometrical av-erage of both measurements.

For each sample and each direction the sample size was n = 10.

All calculations was made in agreement with formula of PN -73/P0463.

ASTM D 4032 92, Standard test method for measuring fabric stiffness by the circular bend procedure [22]This is a method of multidirectional force action to a specified strain. Its principle of measurement consists in determining the maximal force of a mandrel causing a simultaneous multidirectional fabric strain by pushing a sample through the tester table hole. Stiffness measurements according to this method were performed by means of a digital pneumatic.

Table 2. Structural parameters of the knit-ted fabrics tested.

Symbol of knitted

fabric group

Porosity Paverage value, %

Max clearance surface

Cs max., mm2

I 46.6 0.14II 35.3 0.05III 55.7 1.70IV 69.1 1.91V 50.9 4.77VI 65.2 3.12VII 73.9 1.04VIII 71.0 0.89IX 74.8 1.19X 71.2 0.86 Figure 3. Scheme of measurement by the loop method; 1) clamps, 2) measuring

scale, 3) fabric sample, m) loop length [11].

Figure 4. Digital pneumatic stiffness tester [23].

Figure 5. Operating principle of UDM-1 instrument.

1

2

3 m

Stationary beam

Sample in clamps

Mobile beam

Vibration induction system

OscillographFrequency

meter

Low frequency generator

Digital gage

Plunger

Platform + sample

FIBRES & TEXTILES in Eastern Europe 2014, Vol. 22, No. 1(103)46

On the Oscillograph one can see the moment when resonance is reached.

The elasticity modulus Ed is calculated from the following formula:

Ed 20

24ScTp

Mlld = , N/m2 (6)

where: l0 - operating sample length in m, l - load weight in kg, Sc - surface of sample cross-section in m2, - vibra-tion period corresponding to resonance moment in s.

The bending stiffness Rb can be deter-mined using the formula of bending stiff-ness:

Rb = Ed.I, Nm2 (7)

The moment of inertia I for a rectangular sample cross-section amounts to:

12

3bhI = , m4 (8)

where: b - sample width, h - sample thickness.

Measurements are carried out on rec-tangular samples of width = 30 mm and length = 100 mm cut out in lon-gitudinal and transversal directions, and at an angle of 45. The load mass MI = 0.0407 kg. The measurement result is an average value of sample size n = 15.

The calculations were performed in ac-cordance with the methodology set [27].

The program developed for mathemati-cal processing, which is linked to the ap-paratus, allows one to analyse the elas-ticity modulus in each direction (multi-directionally), within an angle range of 0 - 360, using the interpolation method [26].

This processing results in a polar dia-gram of modulus Ed as a function of the inclination angle (angle between the samples axis and the direction of vibra-tion). The representation of Ed = f (angle) within the range of 0 - 360 in the form of a linear diagram shows that in view of the mirror reflections of curves in succes-sive ranges of the polar diagram, it is enough to analyse the variability of Ed values or angles at 0 90. Ed assessment takes into account the anisotropic proper-ties of textiles. Figure 6 shows examples of polar and linear diagrams.

In the method described above, the result of stiffness assessment consists of the av-eraged Ed values for the basic directions (longitudinal, transversal and bias direc-tion - 45 (deg) to the samples axis) and the polar diagram.

Statistical analysis Statistical procedures were carried out with the use of the STATISTICA 8 pro-gram [29].

The following tests were performed:n Descriptive statistics M - mean, SD

- standard deviation, SV coefficient of variation, shape of distribution nor-mality

n Analysis of variance:

n one-way ANOVA, a technique used to compare the means of groups (ten groups of knitted fabrics)

n post hoc statistics in groups, results of multiple comparisons peer-to-peer (45 pairs of groups). Signifi-cant difference between pairs at the level = 0.05 ; tests for distribution normality RIR Tukeys; without normal distribution Krusk-Wal-lis H.

n Spearmans rank correlation

To check the comparability of results of the methods analysed Spearmans rank correlation coefficients between stiffness results of the methods were calculated.

n Test power analysis. Performing pow-er analysis and sample size estimation is an important aspect of experimental results [29 - 32] The power of a test is determined by three factors: the sam-ple size, level, and effect size. The levels of effect size determined by Co-hen [31, 32] and used for test power calculation are listed in Table 3.

Figure 6. Diagrams of Ed as a function of the inclination angle of the samples axis to the direction of vibration (sample VII).

Table 3. Levels of effect size.

Effect sizePower levels

Small Medium LargeNormal distributionf-tests ANOVA 0.10 0.25 0.40

Without a normal distributiont-test on means

0.20 0.50 0.80

Warp

Weft

Angle 45

0 90 180 270 360Inclination angle,

0 - 9090 - 180180 - 270270 - 360

25

20

15

10

5

0

Ed,

MP

a

bh3

12

47FIBRES & TEXTILES in Eastern Europe 2014, Vol. 22, No. 1(103)

The test power for the groups analysed was calculated using level = 0.05; effect sizes at a medium and large level of power; tests for distribution normality f - Anova test; without normal distribu-tion - t-test on means.

The test power for the sample size of the methods was calculated and the number of measurements required for the accept-able test power level 0.8 0.9 was ana-lysed [31, 32].

Analysis of the variability of directional bending stiffness based on the diagrams EdUsing the possibility of presenting the val-ues of elasticity modulus (Ed) (UDM-1) in the form of a diagram comprising the whole range of the force direction 0 - 90, an additional analysis of the mod-ulus as a function of the direction of the force was made.

n Results and discussionStatistical analysisBasic descriptive statistic parametersThe test results of bending stiffness and the basic descriptive statistic parameters are listed in Table 4.

Test of normality distribution show that only method UDM-1 has a normality shape of distribution.

Analysis of varianceOne-way ANOVA. In the results of the analysis of variance at the level of prob-ability p < 0.05, marked effects were significant. It means that the averages of groups differ significantly.

Post hoc statistics in groups, multiple comparisons peer-to-peer. Analysis of results of multiple comparison peer-to-peer (45 pairs of groups) tests show that significant differences occur only in 40 - 50% of all the groups tested. Among the methods under comparison, it is the UDM-1 (Rb) method that better differen-tiates the groups tested than the remain-ing two methods.

The results of multiple comparisons by RIR Tukeys test and Krusk-Wallis H. test are listed in Table 5.

Analysis of these results shows that significant differences occur only in 40 - 50% of all the groups tested. Among the methods under comparison, it is the UDM-1 (Rb) that better differentiates

Table 4. Test results of bending stiffness.

Symbol of knitted fabric group

PNG, mNm; n = 20

ASTMF, N; n = 10

UDM-1Rb, Nm2, n = 15

M SD CV,% M SD CV,% M SD CV, %I 8.02 0.61 7.60 1.67 0.05 3.50 2.39 1.22 51.0II 4.81 1.50 31.2 1.73 0.05 14.3 3.00 2.55 84.9III 3.28 0.44 13.4 1.52 0.18 12.1 2.02 1.13 56.0IV 3.77 0.50 13.3 1.52 0.22 14.8 0.91 0.65 71.1V 3.71 0.53 14.3 1.35 0.10 7.50 2.49 0.68 27.6VI 3.08 0.37 12.0 1.40 0.31 23.4 2.16 1.23 56.9VII 2.11 0.38 18.0 0.51 0.13 26.1 0.56 0.20 37.3VIII 2.29 0.27 11.8 0.59 0.13 22.0 0.51 0.13 26.4IX 1.79 0.76 42.5 0.51 0.11 21.8 0.47 0.49 104X 2.08 0.25 12.0 0.58 0.13 22,0 0.56 0.57 102

Table 5. Results of multiple comparisons (45 pairs of groups). Significant difference be-tween pairs at the level p = 0.05.

Method Significant differences in number of pairsSignificant differences

of all the groups tested, %

PN 18 40

ASTM 18 40 UDM-1 23 50

Figure 7. Results of Spermans rang correlation between methods compared.

a)

b)

c)

FIBRES & TEXTILES in Eastern Europe 2014, Vol. 22, No. 1(103)48

the groups tested than the remaining two methods.

Spearmans rank correlationConsidering the different indicators and value level of the methods under analy-sis, Spearmans rank correlation was used for their comparison. The results of Spearmans rank correlation coefficients are shown in Figure. 7. This graphs

Table 6. Results of power test analysis.

Level of power PN ASTM UDM-1

Sample size, n 20 10 15

Effect sizeMedium t = 0.50 f = 0.25Large t = 0.80 f = 0.40

Power calculatedMedium 0.15 0.09 0.45Large 0.31 0.17 0.98

Sample size required, nMedium 189 189 37Large 74 74 15

Figure 8. Image of diagrams for various groups of knitted fabric stitch: a) plain, double needle board stitches (velvet, chain), b) plain stitch, double needle board with a network structure; c) V, VI plain, three needle board stitch with a network structure; VII, VIII plain, double needle board stitch.

I II

III

IX X

V VI

VII VIII

IV

49FIBRES & TEXTILES in Eastern Europe 2014, Vol. 22, No. 1(103)

show that a high level of correlation co-efficients, R > 0.7, between all methods compared means that they give compa-rable revaluation of the bending stiffness of the fabrics tested. It is suitable to com-pare estimates of bending stiffness for re-sults Rb, G and F but only in a specified range.

Test power analysis Results of the test power calculated at the acceptance level of effect size (STATISTICA 8 program) are presented in Table 6.

This results show that only the UDM-1 method reached a satisfactorily large lev-el of test power - 0.9088 and has a suffi-cient sample size n = 15. Residual meth-ods did not achieve satisfactory results of power - 0.8 - 0.9 at a large and medium level and could not bring results with a statistically significant difference. On the other hand the required sample size cal-culated for the standardised methods is difficult to use in practice.

Analysis of the variability of the directional bending stiffness based on the diagrams Ed Diagrams of all the samples tested are shown in Figure 8.

The presentation of diagrams Ed as a function of the axis slope of the sample to the direction of force action allows one to isolate some groups corresponding to the stitch of the nets tested and to compare them within these groups. The shape of curves depends on the repeat determining stitch, clearance size, yarn thickness and structure.

Knitting of the first groups I and II, (Fig-ure 1, Table 2) with combined stitches (chain, velvet) shows increasing stiff-ness versus the angle up to the maximal double Ed value for the parallel direction to wales (90). At the same time, these groups show the greatest anisotropy of stiffness.

In the case of groups with plain net stitches, values of the elasticity modulus are sinusoidally changed, reaching their maximum within the range of 30 - 50.

Analysing these diagrams, one can as-sess the character of bending stiffness for the specified fabric stitch on the basis of modulus values. Knitting with combined stitches (I and II) is characterised by the greatest stiffness among the knitting test-

ed, which is shown at about 90, i.e. in the direction of wales.

Groups with plain two-needle net stitches (III, IV, IX and X), Figure 8.b reach their maximal stiffness within the range of 30 - 60.

Groups with plain three-needle and two-needle stitches and with different yarns and numbers of knitted loops (V, VI, VII and VIII), Figure 8.c constitute nets with the best multi-directionally equalised stiffness due to the smallest differences in the modulus versus the angle.

n Conclusions The aim of this work was to compara-tively evaluate three selected testing methods using different measurement principles and choose the best to evalu-ate the bending stiffness of net-like warp knitted fabrics. The experimental de-sign included unidirectional force action (PN-73/P0431) and multidirectional force action (ASTM-D 4032-94) as well as bending stiffness testing by direct determination of Youngs modulus (E) used for calculations of bending stiffness (method UDM-1). Comparison of results and evaluating properties of the methods was carried out by means of statistical tests with the use of the STATISTICA 8 program.

Results of the analysis of variance show that the one-way ANOVA for the three methods tested confirmed differences between the average values of bending stiffness for all the groups. Results of multiple comparisons peer-to-peer show that significant differences occur only in 40-50% of all the groups tested. Among the methods under comparison, it is the UDM-1 (Rb) that better differentiates the groups tested than the remaining two . The high level of Spearmans rank cor-relation coefficients, R > 0.7, between all methods compared is well suited to com-pare estimates of bending stiffness for results Rb, G and F, but only in a speci-fied range. Results of the test power show that only the UDM-1 method reached a satisfactorily large level of test power 0.9088 and has sufficient sample size n = 15. Standardised methods in PN and ASTM did not achieve satisfactory re-sults of power 0.8 - 0.9 at a large and me-dium level, and the required sample size calculated for them is difficult to use in practice. Analysing the variability of the directional bending stiffness based on the

diagrams (Ed), one can assess the char-acter of bending stiffness anizotropy for the specified fabric stitch on the basis of modulus values. In a general summary it can be concluded that standardised meth-ods in PN and ASTM, as a comparison, can be used in quality control, applicable in industry. Due to the possibility of anal-ysis diagrams in many directions of force action and the satisfactorily large level of test power, the UDM-1 method is useful for scientific works.

AcknowledgmentsThe samples of knitted fabrics with a network structure used in this study were prepared within research project 1242/T08 29 (2005-2008). The authors would like to thank Krzysz-tof Raczyski, M.Sc., Project Manager, for providing the material for investigations. The authors are also indebted to Irena Kamiska, M.Sc. for performing microscopic analyses of the fabric structure.

References 1. yliski T. Metrologia Wkiennicza.

WNT, 1965: 403 410. 2. Dziworska G. Przegld modeli, system-

w i metod pomiarowych sztywnoci zgi-nania paskich wyrobw wkienniczych. Przegld Wkienniczy 2004; 8: 40-43.

3. Ostwald M. Podstawy wytrzymaoci materiaw. WPP, 2007: 93 98.

4. yliski T. Nauka o Wknie. WPLiS 1958: 131 161.

5. Urbaczyk GW. Fizyka Wkna 2002: 144 196.

6. Kocik M, urek W, Krucinska I, et al. Evaluating the Bendig Rigidity of Flat Textiles with the Use of an Instron Ten-sile Tester. Fibres & Textiles in Eastern Europe 2005; 2: 31-34.

7. ASTM D4850-03a. Standard Terminol-ogy Relating to Fabrics.

8. ASTM D1388-96. Standard Test Method for Stiffness of Fabrics.

9. BS 3356:1990. Method for the deter-mination of bending lenght and flexural rigidity of fabrics.

10. ISO 9073-7.1998. Test methods for non-wovens. Determination of Bendig lenght.

11. PN-73/P-04631. Metody bada wyrobw wkienniczych. Wyznaczanie sztywno-ci zginania. Methods of test for textiles. Determination of bending stiffness.

12. Brown P. Measurment of Single Jersey Fabric Stiffness: A Simple Method. Text. Res. J. 1978: 295-299.

13. Szablewski P, Kobza W. Numeryc-zna analiza testu Pierca okrelajcego sztywno zginania wyrobw wkien-niczych. Przegld Wkienniczy 2002; 70: 14 -17.

14. ASTM D5732-95. Standard Test Method for Stiffness of Nonwoven Fabrics Using the Cantilever Test.

15. Ghane M, Saghafi R, Zarrebini M, Sem-nani D. Evaluation of Bending Modulus of Needle-Punched Fabrics Using Two Simply Supported Beam Method. Fibres

FIBRES & TEXTILES in Eastern Europe 2014, Vol. 22, No. 1(103)50

& Textiles in Eastern Europe 2011; 19, 4 (87): 89-93.

16. Weia M. The Theory of the Cantilever Stiffness Test. J. Textile Inst. 1998; 80: 98 106.

17. ASTM D6828-02. Standard Test Method for Stiffness of Fabric by the Blade/Slot Procedure.

18. Kalyanaraman AR, Sivaramakrishnan A. An electronic Fabric Stiffness Me-ter -Performance Evaluation with the Known Instruments. Text. Res. J. 1984; 21: 479-484.

19. Abbott NJ. The Measurement of Stiff-ness in Textile Fabrics. Text. Res. J. 1951; 21: 435-441.

20. Sun MN. New Tester and Method for Measuring Fabrics Stiffness and Drape. Text. Res. J. 2008; 78: 761-770.

21. De la Araujo M, Fangueiro R, Soutinho F. Improving the stiffness of unidirec-tionally oriented weft-knitted structures for polymer matrix composite reinforce-ment. J. Textile Ins. 2009; 9: 715-721.

22. Harrabi L, Dolez PI, Vu-Khanh T, et al. Characterization of protective Glover stiffness: Development of a multidirec-tional deformation test method. Safety Science 2008; 46: 10251036.

23. ASTM D4032-94. Standard test Method for Stiffness of Fabrics by the Circular Bend Procedure.

24. Vlasenko V, Kovtun S, Bereznenko N. Investigation of Composite Textiles Visco-elastic Properties by Methods of longitudal Resonance Vibration. In: 4th Central European Conference Fibre-Grade Polymers, Chemical Fibres and Special Textiles. Czech Republic 2005; 7-9 September, 217-8.

25. Owaki H. Measuring Flexural Rigidity of Fabrics by a Vibrating Disk Method. J The Text Mach Soc Japan 1968; 12: 40-43.

26. Ajeli S, Rastgo A, Gorga RE. An analysis of the bending rigidity of warp-knitted fabrics: a comparision of experimental results to a mechani-cal model. J. Textile Inst. 2009; 6: 496-506.

27. Kostrickij WW. Mietodika i ispitatielnaja ustanowka dla issliedowania dinamic-zeskich swojstw polimernych plienoc-znych materiaow i wookon. Zawodska-ja aboratorija 1990; 56: 38-42.

28 Wiecek T, Konecki W. Comparative Re-search of the Dynamic Youngs Module. Fibres Fibres &Textiles in Eastern Eu-rope 2011; 19, 4(87): 89-93.

29. Program Stat Soft Statistica 8. 30. Stat Soft. Inc. Electronic Statistics Tex-

book. Tulsa, OK.: Statsoft. WEB, //www.statsoft. com/textbook/ 2010.

31. Cohen J. Statistical power analysis for the behavioral sciences. Hillsdale, NJ: Lawrence Erlbaum Associates 1998; 130-380.

32. Power Analysis, Univresity of Visconsin Madison, http://psych.visc.edu/henr-iques.power.html

33. Grabowska B, Karaszewska A, Kamiska I. Badanie sztywnoci zgina-nia dzianin osnowowych o strukturze siatki (in Polish). In: IX Miedzynarodowa Konferencja Naukowo Techniczna Knitt Tech. Rydzyna, 19.06.2010.

Received 14.03.2013 Reviewed 17.09.2013

INSTITUTE OF BIOPOLYMERS AND CHEMICAL FIBRES

LABORATORY OF BIODEGRADATION

The Laboratory of Biodegradation operates within the structure of the In-stitute of Biopolymers and Chemical Fibres. It is a modern laboratory with a certificate of accreditation according to Standard PN-EN/ISO/IEC-17025: 2005 (a quality system) bestowed by the Polish Accreditation Centre (PCA). The laboratory works at a global level and can cooperate with many institu-tions that produce, process and investigate polymeric materials. Thanks to its modern equipment, the Laboratory of Biodegradation can maintain coopera-tion with Polish and foreign research centers as well as manufacturers and be helpful in assessing the biodegradability of polymeric materials and textiles.

The Laboratory of Biodegradation as-sesses the susceptibility of polymeric and textile materials to biological degradation caused by microorganisms occurring in the natural environment (soil, compost and wa-ter medium). The testing of biodegradation is carried out in oxygen using innovative methods like respirometric testing with the continuous reading of the CO2 delivered. The laboratorys modern MICRO-OXYMAX RESPIROMETER is used for carrying out tests in accordance with International Standards.

The methodology of biodegradability testing has been prepared on the basis of the following standards:

n testing in aqueous medium: Determination of the ultimate aerobic biodegrability of plastic materials and textiles in an aqueous medium. A method of analysing the carbon dioxide evolved (PN-EN ISO 14 852: 2007, and PN-EN ISO 8192: 2007)

n testing in compost medium: Determination of the degree of disinterga-tion of plastic materials and textiles under simulated composting condi-tions in a laboratory-scale test. A method of determining the weight loss (PN-EN ISO 20 200: 2007, PN-EN ISO 14 045: 2005, and PN-EN ISO 14 806: 2010)

n testing in soil medium: Determination of the degree of disintergation of plastic materials and textiles under simulated soil conditions in a laborato-ry-scale test. A method of determining the weight loss (PN-EN ISO 11 266: 1997, PN-EN ISO 11 721-1: 2002, and PN-EN ISO 11 721-2: 2002).

The following methods are applied in the as-sessment of biodegradation: gel chromatography (GPC), infrared spectroscopy (IR), thermogravi-metric analysis (TGA) and scanning electron mi-croscopy (SEM).

Contact:

INSTITUTE OF BIOPOLYMERS AND CHEMICAL FIBRESul. M. Skodowskiej-Curie 19/27, 90-570 d, Poland

Agnieszka Gutowska Ph. D., tel. (+48 42) 638 03 31, e-mail: [email protected]

AB 388

Popular Tags:

Click here to load reader

Embed Size (px)

Recommended